|Year : 2022 | Volume
| Issue : 1 | Page : 5
Cytotoxicity effect of orthodontic miniscrew-implant in different types of mouthwash: An in-vitro study
Wulan S Utami1, Haru S Anggani2, Maria Purbiati2
1 Orthodontics Residency Program, Faculty of Dentistry, Universitas Indonesia, Jakarta, Indonesia
2 Department of Orthodontics, Faculty of Dentistry, Universitas Indonesia, Jakarta, Indonesia
|Date of Submission||30-Jun-2021|
|Date of Decision||14-Oct-2021|
|Date of Acceptance||21-Oct-2021|
|Date of Web Publication||28-Jan-2022|
Haru S Anggani
Jalan Salemba Raya No. 4, Jakarta Pusat
Source of Support: None, Conflict of Interest: None
CONTEXT: Orthodontic miniscrew implants (OMIs) are widely used as anchorage alternatives, but recent studies revealed the corrosion behavior of OMIs when they come in contact with mouthwashes. The corrosion materials that are released can cause toxicity, allergy, and mutagenicity.
AIMS: This study aims to analyze the cytotoxicity effects of OMIs exposed to different types of mouthwash using human gingival fibroblast (HGFs).
SETTINGS AND DESIGN: Experimental laboratory research.
METHODS AND MATERIAL: Twenty-eight samples of Ti alloy OMIs immersed separately in four groups of different types of mouthwash (chlorhexidine gluconate 0.2% mouthwash (CHX), fluoridated (sodium fluoride 0.2%) mouthwash, chitosan mouthwash 1.5%, and aquadest) for 28 d. Elution of each group and the mouthwash itself were added to the cell culture and incubated for 24 h. Changes in cell viability were performed by MTT Assay.
STATISTICAL ANALYSIS USED: Data were tested for normality with Shapiro–Wilk, homogeneity with Levene test, and analyzed using an independent T-test (P < 0.05).
RESULTS: The differences between the cytotoxicity of the elution of MIO and the mouthwash solution itself in the group of CHX and Fluoride were statistically significant (P < 0.05). No significant differences were found in the group of chitosan and aquadest (P > 0.05).
CONCLUSIONS: The 1.5% chitosan mouthwash can be offered to patients with Ti alloy-based OMIs rather than the 0.2% chlorhexidine gluconate and 0.2% sodium fluoride mouthwashes.
Keywords: Chitosan, chlorhexidine, cytotoxicity, mouthwash, orthodontic mini-implant, Ti alloy
|How to cite this article:|
Utami WS, Anggani HS, Purbiati M. Cytotoxicity effect of orthodontic miniscrew-implant in different types of mouthwash: An in-vitro study. J Orthodont Sci 2022;11:5
|How to cite this URL:|
Utami WS, Anggani HS, Purbiati M. Cytotoxicity effect of orthodontic miniscrew-implant in different types of mouthwash: An in-vitro study. J Orthodont Sci [serial online] 2022 [cited 2022 Sep 27];11:5. Available from: https://www.jorthodsci.org/text.asp?2022/11/1/5/336721
| Introduction|| |
Biomaterials used in dentistry, or orthodontics particularly, must have good biocompatibility. Ti alloy is one of the materials currently used for orthodontic miniscrew-implants (OMIs) or temporary anchorage devices (miniscrews). Miniscrews are orthodontic devices that are used as an intraoral skeletal anchorage. This compliance-independent device is known to be easy to install and remove, relatively affordable, and able to provide absolute anchorage.,
Chlorhexidine and fluoride mouthwashes are common choices of mouthwash used to maintain oral health in orthodontic patients., However, several studies have reported the effect of the exposure of both types of mouthwash on the properties and biocompatibility of orthodontic appliances, including miniscrew implants.,, A study using scanning electron microscopy (SEM) also stated that fluoride mouthwash could cause corrosion in the form of crevices and pits on the surface of miniscrews after 28 d of immersion. These findings need some attention because the use of mouthwashes is often recommended for patients to maintain their oral health.
Chitosan, on the other hand, as a natural biomaterial has been studied as an alternative mouthwash because of its antibacterial properties and biocompatibility.,,, Its antibacterial activity against total bacteria and E. faecialis has been found to be comparable to chlorhexidine mouthwash., Therefore, this study sought to evaluate the cytotoxicity effect of miniscrews exposed to different types of mouthwash using human gingival fibroblast (HGFs).
| Subjects and Methods|| |
Miniscrews used in this study were dual-top composed of Ti alloy (Ti6Al4V), (Jeil Medical, Korea). The four types of solutions used are commercially available: 0.2% digluconate mouthwash (MINOSEP®, PT. Minorock Mandiri, Depok, Indonesia), 0.2% sodium fluoride mouthwash (Pepsodent Pro Complete, Unilever, Indonesia), 1% chitosan with 0.25% acetic acid (KITOBETM, Berkah Inovasi Kreatif Indonesia, Bogor, Indonesia), and aquadest (Aqua Pro Injection Sterile, PT. Ikapharmindo Putramas, Jakarta, Indonesia). This protocol was approved by Ethics Committee of Research at the Faculty of Dentistry, Universitas Indonesia, Jakarta, Indonesia (ref. No. 11/Ethical Approval/FKGUI/VII/2020 Date of approval: 21-July-2020.
Preparation of eluates from miniscrews
Each type of treatment solution (n = 7) was randomly filled in Eppendorf tubes and randomly labeled as red, blue, green, and yellow by the first author's supervisor.
The amount of solution was calculated by the ratio of 1 mL for 0.2 g of miniscrew weight according to DIN ED ISO 10271. Twenty-eight specimens of eluates were obtained by individually immersing miniscrews in 385 μl of each type of treatment solution (seven eluates of miniscrews in each type of solution) and incubated for 28 d at 37°C [Figure 1]. Each type of treatment solution without TAD was also incubated for 28 d as a control group.
|Figure 1: Preparation of eluates from miniscrews in different types of mouthwash|
Click here to view
Human primary gingival fibroblast cell culture
Human primary gingival fibroblast (HGF) cells were obtained from the stored biological material of the previous study. The cells were cultured in alpha-modified eagle medium (α-MEM) pH 7.2 (Gibco, Grand Island, NY, USA) with 10% of fetal bovine serum (FBS) (Biosera, UK), 100 U/ml penicillin, 100 μg/ml streptomycin, and 1% amphotericin B (Gibco, Grand Islan, NY, USA). Cultures were maintained at 37°C, 5% CO2, and 95% air until reach 70%–80% confluence [Figure 2].
|Figure 2: Human gingival fibroblast cells (HGFs), initial stage (left) and after reached 80% confluence (right)|
Click here to view
In vitro cytotoxicity by MTT assay
Aliquots of 100 μl of HGF cell suspension (4 × 104 cells/well) were pipetted into 96-well flat-bottom plates (Corning Costar Corporation, Cambridge, MA, USA) and incubated for another 48 h to obtain a cell monolayer. After the monolayer growth was confirmed by an inverted light microscope, the culture medium was removed and 20 μl of each eluate or 20 μl of each treatment solution with 100 μl of fresh culture medium were added to the correspondent well. Each eluate was tested in quadruple and incubated at 37°C, 5% CO2, and 95% air for 24 h. Aliquots of 20 μl 2% chlorhexidine gluconate solution and an additional 20 μl of the medium culture were also added to the well as positive and negative control, respectively [Figure 3].
|Figure 3: Configuration of the 96-well flat-bottom plates. Eluates of Miniscrews on the treatment solutions; (A) 0.2% Chlorhexidine gluconate mouthwash, (B) 1% Chitosan solution, (C) Aquadest, (D) 0.2% Sodium fluoride mouthwash. 2% chlorhexidine gluconate as positive control (P) and complete medium without treatment solution as negative control (N)|
Click here to view
After 24 h, the toxic effect of miniscrews exposed in the mouthwashes was tested against the mouthwash itself by 3-(4,5-dimethylthiazol-2-yl) 2,5-diphenyltetrazolium bromide (MTT) assay. 10 μl aliquots of MTT solution (5 mg/ml) were added to each well and incubated for another 3 h at 37°C, 5% CO2, and 95% air. Next, 100 μl of acidified isopropanol (HCL and isopropanol) were added to dissolve the formazan crystals and the absorbance was read by using an enzyme-linked immunosorbent assay (ELISA) plate reader at 600 nm. The percentage of cell viability was calculated as
All data were processed in Excel and tested with the Statistical Package for Social Science (SPSS) version 23.0 software program (IBM Corp., Armonk, NY, USA). Percentage of cell viability in each group was tested for normality with Shapiro–Wilkis test and homogeneity with Levene test. The difference in the percentage of cell viability between the eluates and the treatment solutions in the chlorhexidine, fluoride, chitosan, and aquadest groups were tested using an independent T-test. Statistical significance was determined at the level of P < 0.05.
| Results and Discussion|| |
There are four groups of cytotoxicity based on the percentage of cell viability, namely not cytotoxic if there are more than 90% of cells that are viable, mild cytotoxic if 60%–90% of viable cells are found, moderate cytotoxic if 30%–59% of viable cells are obtained, and severe cytotoxicity when less than 30% of cells are viable.
The four test solutions without OMI immersion showed different toxicities [Table 1]. Aquadest and 1.5% chitosan solution showed less than 30% toxicity, meaning that aquadest and 1.5% chitosan solution were not toxic to gingival fibroblasts. This is in accordance with previous research by Chellat et al. that chitosan does not show toxicity in fibroblast cell lines. This finding is different from the research of Uğur Aydin et al., which revealed a moderate toxic effect of chitosan solution on gingival fibroblast cell line. The possibility of the differences in these results is due to the greater concentration of the chitosan solution used as well as the different test methods.
A solution of 0.2% chlorhexidine and 1.5% fluoride (sodium fluoride 0.2%) was found to be highly toxic to gingival fibroblast with cell viability of less than 30%. The toxicity of the two solutions has been a concern in recent decades. Chlorhexidine was found to be toxic to gingival fibroblast cells, and several other cells, as well as fluoride which was also found to be toxic to gingival fibroblasts with the level of toxicity depending on the concentration and time of exposure.
The four test groups in this study showed an increase in the toxicity of the mouthwashes [Figure 4]. The increase in toxicity is most likely due to the toxic effect of the release of OMI Ti alloy metal ions in the mouthwashes due to decreased resistance of OMI. The released metal ions can induce toxic effects depending on the type, size, and concentration. Okazaki et al. in their research revealed that the concentration of aluminum ions 0.2–0.5 ppm and 0.002–0.2 ppm vanadium in the culture medium could significantly decrease the viability of L929 and MC3T3-E1 cells, while the concentration of Ti ions was 0.2–0.3 ppm in the medium culture is not toxic to the two cells. Another study revealed that Ti ions are toxic at concentrations of more than 11 ppm in the culture medium. However, we cannot conclude the relationship between the type and concentration of metal ions released and the toxicity of gingival fibroblast cells in this study. This can be further investigated by quantitatively evaluating the number and types of metal ions released in the test solution by using the inductively coupled plasma-optical emission spectrometry (ICP-OES) method.
|Figure 4: Cell damage caused by solution without TADs (blue) and caused by elution or solution conditioned by miniscrews for 28 d (orange). (*): Cell survival was significantly decreased in chlorhexidine and fluoride groups (P < 0.05)|
Click here to view
Two test groups in this study showed a significant increase in toxicity, which are the 0.2% chlorhexidine gluconate solution and 0.2% fluoride solution. This result is in line with the research of Quaranta et al., which showed the effect of exposure to 0.2% chlorhexidine mouthwashes on Ti alloy in the form of signs of corrosion on Ti alloy discs when associated with OMI corrosivity. The electrochemical study by Bhola et al. revealed that chlorhexidine 0.1% can increase the corrosivity of the Ti material by increasing the dissolution of the Ti oxide protective layer. In addition, chlorhexidine can bind with chloride ions, which can hinder the process of repassivation of the protective layer of the Ti material.
The increase in toxicity in the fluoride group in this study is thought to be closely related to the ability of fluoride ions to damage the TiO2 protective layer of Ti alloy. This finding is in line with the SEM research by Aboodi et al. which shows that fluoride solution can trigger corrosion of OMI Ti alloy in the form of signs of corrosion in the form of dots and niches. Previous research by Anwar et al. regarding the effect of fluoride on the corrosion properties of cpTi and Ti alloy dental implants also revealed that the use of fluoride therapy (NaF) above 0.1 M could significantly decrease the corrosion resistance of Ti and Ti alloy. Huang et al. also revealed that the higher the fluoride content in a mouthwash, the lower the corrosion resistance of Ti alloy. This study used a 0.2% sodium fluoride mouthwash, which was the standard concentration and was sufficient to significantly increase the toxic effect of OMI Ti alloy. The phenomenon of corrosion of Ti alloy in fluoride solution is described by the formation of dissolved Ti–F complexes in the form of Na2TiF6 or in the form of TiCl6 and TiF6, which leads to a decrease in the resistance of the protection layer.
Immersion of OMI Ti alloy in aquadest and chitosan solution did not significantly increase the toxicity. This is in accordance with several previous studies which proved that Ti alloy was not toxic and did not cause a decrease in the viability of gingival fibroblast cells with the extraction medium of culture medium and saline solution., Toxicity of OMI immersed in aquadest and chitosan solution (95.91% and 93.97%) in this study was slightly larger than those found in the research of Finke et al., which was 89.4%. Although using the same OMI brand, this difference may occur due to differences in the extraction medium and cell types used. This study by Finke et al., used a culture medium (α-MEM) as an extraction media with gingival fibroblast cell line, whereas this study used gingival fibroblast primary cells.
Nonetheless, the results of this study must be interpreted with caution because like other in vitro studies, it does not describe the actual condition of the mouth. The results obtained may show lower toxicity than the actual oral conditions due to the presence of saliva as a buffer. In contrast, it can also show higher than actual toxicity, probably due to the dynamic conditions of the oral cavity with varying salivary pH and oral temperature.
This study shows that the elution of OMI Ti alloy in chlorhexidine and fluoride mouthwashes can increase its toxic effect on gingival fibroblasts. This study also showed that OMI Ti alloy elution in aquadest and chitosan solution was not toxic to gingival fibroblasts. This finding can provide added value in the development of chitosan solution as a mouthwash for patients with OMI Ti alloy or other Ti alloy-based devices, apart from its effectiveness which is also still under development.
| Conclusion|| |
- The 0.2% chlorhexidine gluconate and 0.2% sodium fluoride mouthwashes are highly toxic to HGF cell cultures, while the 1.5% chitosan solution and aquadest are not toxic to HGF cell cultures.
- Miniscrews significantly increased the toxicity of the 0.2% chlorhexidine gluconate and 0.2% sodium fluoride mouthwashes to HGF cell cultures, but it did not increase the toxicity of 1.5% chitosan solution and aquadest.
Financial support and sponsorship
Universitas Indonesia through PUTI Grant with contract number NKB-2345/UN2.RST/HKP. 05.00/2020.
Conflicts of interest
There are no conflicts of interest.
| References|| |
Jasoria G, Shamim W, Rathore S, Kalra A, Manchanda M, Jaggi N. Miniscrew implants as temporary anchorage devices in orthodontics: A comprehensive review. J Contemp Dent Pract 2013;14:993-9.
Bajaj R, Shenoy U, Banerjee S, Hazare A, Karia H, Atulkar M. Implants in orthodontics- A brief review. Int J Oral Heal Med Res 2017;3:92-7.
Cortizo MC, Oberti TG, Cortizo MS, Cortizo AM, Fernández Lorenzo De Mele MA. Chlorhexidine delivery system from titanium/polybenzyl acrylate coating: Evaluation of cytotoxicity and early bacterial adhesion. J Dent 2012;40:329-37.
Srivastava K, Tikku T, Khanna R, Sachan K. Risk factors and management of white spot lesions in orthodontics. J Orthod Sci 2013;2:43-9.
Mandsaurwala M, Kalia A, Gupta G, Hegde A, Mirdehghan N. Comparative evaluation of ion release from orthodontic mini-implants in 2 mouthwashes: An in-vitro study. Int J Oral Heal Dent 2015;1:177-81.
Alves CBC, Segurado MN, Dorta MCL, Dias FR, Lenza MG, Lenza MA. Evaluation of cytotoxicity and corrosion resistance of orthodontic mini-implants. Dental Press J Orthod 2016;21:39-46.
Abbassy M. Fluoride influences nickel-titanium orthodontic wires′ surface texture and friction resistance. J Orthod Sci 2016;5:121-6.
Aboodi H, A-Dabagh DJN. Analysis of two different types of orthodontic mini-implants immeres in fluoridated mouthwashes using scanning elextron microscopy (SEM). PLoS One 2019;14:1-17.
Younes I, Sellimi S, Rinaudo M, Jelouli K, Nasri M. Influence of acetylation degree and molecular weight of homogenous chitosans on antibacterial and antifungal activities. Int J Food Microb 2014;185:57-63.
Hasriati E, Anggani HS, Purbiati M, Bachtiar EW. Antibacterial effect of 0.2% chlorhexidine and 1% chitosan mouthwash on bacteria during orthodontic miniscrew use. Int J Appl Pharm 2020;12:8-12.
Husain S, Al-Samadani KH, Najeeb S, Zafar MS, Khurshid Z, Zohaib S, et al
. Chitosan biomaterials for current and potential dental applications. Materials (Basel) 2017;10:1-20. doi: 10.3390/ma10060602.
Costa E, Silva S, Costa M, Pereira M, Campos DA, Odila J, et al
. Chitosan mouthwash: Toxicity and in vivo
validation. Carbohydr Polym 2014;111:385-92.
Simanjuntak PA, Djauharie N, Nursasongko B. Antibacterial effectiveness of 2% chitosan and 2% chlorhexidine against enterococcus faecalis in biofilm (Laboratory experiment). Int J Appl Pharm 2019;11:44-8.
Rongo R, Valletta R, Bucci R, Rivieccio V, Galeotti A, Michelotti A, et al
. In vitro
biocompatibility of nickel-titanium esthetic orthodontic archwires. Angle Orthod 2016;86:789-95.
Chellat F, Tabrizian M, Dumitriu S, Chornet E, Rivard CH, Yahia L. Study of biodegradation behavior of Chitosan-Xanthan microspheres in simulated physiological media. J Biomed Mater Res 2000;53:592-9.
Uğur Aydin Z, Akpinar KE, Hepokur C, Erdönmez D. Assessment of toxicity and oxidative DNA damage of sodium hypochlorite, chitosan and propolis on fibroblast cells. Braz Oral Res 2018;32:e119.
Pucher JJ, Daniel C. The effects of chlorhexidine digluconate on human fibroblasts in vitro. J Periodontol 1992;63:526-32.
Mariotti AJ, Rumpf DAH. Chlorhexidine-induced changes to human gingival fibroblast collagen and non-collagen protein production. J Periodontol 1999;70:1443-8.
Li YC, Kuan YH, Lee TH, Huang FM, Chang YC. Assessment of the cytotoxicity of chlorhexidine by employing an in vitro
mammalian test system. J Dent Sci 2014;9:130-5.
Hasani Tabatabaei M, Sadeghi Mahounak F, Asgari N, Moradi Z. Cytotoxicity of the ingredients of commonly used toothpastes and mouthwashes on human gingival fibroblasts. Front Dent 2019;16:450-7.
Okazaki Y, Rao S, Asao S, Tateishi T, Katsuda S, Furuki Y. Effect of Ti, Al, and V concentrations on cell viability. Mater Trans JIM 1998;39:1053-62.
Souza JCM, Apaza-Bedoya K, Benfatti CAM, Silva FS, Henriques B. A comprehensive review on the corrosion pathways of titanium dental implants and their biological adverse effects. Metals (Basel) 2020;10:1-14. doi: 10.3390/met10091272.
Quaranta A, Roncini LF, Carlo F Di, Vozza I, Quaranta M. Electrochemical behaviour of titanium in ammine and stannous fluoride and chlorhexidine 0.2% mouthwashes. Int J Immunopathol Pharmacol 2010;1:335-43.
Bhola SM, Kundu S, Alabbas F, Mishra B, Olson DL. An electrochemical study on chlorhexidine gluconate addition to normal saline for oral implant applications. Int J Electrochem Sci 2013;8:5172-82.
Anwar EM, Kheiralla LS, Tammam RH. Effect of fluoride on the corrosion behavior of Ti and Ti6Al4V dental implants coupled with different superstructures. J Oral Implantol 2011;37:309-17.
Huang GY, Jiang HB, Cha JY, Kim KM, Hwang CJ. The effect of fluoride-containing oral rinses on the corrosion resistance of titanium alloy (Ti-6Al-4V). Korean J Orthod 2017;47:306-12.
Huang HH. Electrochemical impedance spectroscopy study of strained titanium in fluoride media. Electrochim Acta 2002;47:2311-8.
Reclaru L, Meyer JM. Effects of fluorides on titanium and other dental alloys in dentistry. Biomaterials 1998;19:85-92.
Galeotti A, Uomo R, Spagnuolo G, Paduano S, Cimino R, Valletta R, et al
. Effect of pH on in vitro
biocompatibility of orthodontic miniscrew implants. Prog Orthod 2013;14:1-7. doi: 10.1186/2196-1042-14-15.
Malkoç S, Öztürk F, Öreki B, Bozkurt BS, Hakki SS. Real-time cell analysis of the cytotoxicity of orthodontic mini-implants on human gingival fibroblasts and mouse osteoblasts. Am J Orthod Dentofac Orthop 2012;141:419-26.
Finke H, Koos B, Fischer-Brandies H, Es-Souni M. In vitro
biocompatibility of orthodontic miniscrews with human gingival fibroblast and SAOS-2 osteoblast cultures. J Orofac Orthop 2018;79:328-36.
[Figure 1], [Figure 2], [Figure 3], [Figure 4]